microstructured shape memory polymer surfaces with ...skm. microstructured shape memory polymer...
Post on 02-Feb-2021
Embed Size (px)
Microstructured Shape Memory Polymer Surfaces with Reversible Dry Adhesion Jeffrey D. Eisenhaure,† Tao Xie,‡ Stephen Varghese,† and Seok Kim*,†
†Department of Mechanical Science and Engineering, University of Illinois at Urbana−Champaign, Urbana, Illinois 61801, United States ‡The State Key Laboratories of Chemical Engineering, Department of Chemical & Biological Engineering, Zhejiang University, Hangzhou, China, 310027
*S Supporting Information
ABSTRACT: We present a shape memory polymer (SMP) surface with repeatable, very strong (>18 atm), and extremely reversible (strong to weak adhesion ratio of >1 × 104) dry adhesion to a glass substrate. This was achieved by exploiting bulk material properties of SMP and surface microstructuring. Its exceptional dry adhesive performance is attributed to the SMP’s rigidity change in response to temperature and its capabilities of temporary shape locking and permanent shape recovery, which when combined with a microtip surface design enables time-independent control of contact area.
KEYWORDS: dry adhesives, shape memory polymer, reversible adhesion
■ INTRODUCTION Reusable dry adhesives with strong adhesion and a high degree of adhesion reversibility are attractive for a wide range of applications including temporary bonding in domestic and industrial settings, the “feet” of climbing robots, and automated assembly at both macro- and microscale. Both adhesive strength and reversibility come from a combination of bulk and surface material properties, often aided by carefully designed surface micro/nanofeatures.1−4 Because a dry adhesive relies primarily on noncovalent molecular interactions to create its adhesion force, it is important to maximize contact area at the molecular scale. To accomplish this, the adhesive material must be compliant enough to conform closely to the surface of the substrate. However, as the adhesive material becomes more compliant it also becomes more susceptible to failure from crack formation and propagation, leading to lower adhesion. A common strategy to overcome this contradiction is to create arrays of microscopic fibrillar structures on a relatively rigid backing layer;5 the microscopic fibrils are compliant enough to conform to the substrate, whereas the rigidity of the macroscopic structure helps to evenly distribute the load among the contact points, thereby delaying the onset of peeling. Although significant efforts have been made to study and manufacture compliant, hierarchical fibrils for dry adhesives,6 relatively few authors have demonstrated the importance of controlling backing layer rigidity.2,7 One such demonstration was performed using phase changing material as a backing layer, where the effective adhesive strength of the overlying elastomer was shown to increase substantially when rigidly supported.7
A change in elastic modulus can be effected in most polymeric materials by shifting the temperature across the
polymer’s glass transition (Tg). A class of thermosensitive smart materials referred to as shape memory polymers (SMPs) are specifically designed to drastically change their mechanical compliance in this way at a convenient Tg.
8 The change in an SMP’s elastic modulus is accompanied by another very important property from which its name is derived: it is ability to lock itself into an arbitrary “temporary” shape and to then recover its original, “permanent” shape. This ability can be utilized to reversibly change the surface morphology of SMP, leading to switchable surface properties such as dry adhesion.9,10 During an SMP’s transformation from a temporary shape to its permanent shape, the stresses generated during attachment are released, which can serve as a unique built-in adhesion detachment mechanism. Despite these attractive features offered by SMP, strong adhesion has only been previously demonstrated when SMP is combined with an intrinsically adhesive (or sticky) rubber layer or when the surface is treated with adhesion molecules.3,4,11,12 We hereby explore SMP as a single component to construct a strong dry adhesive, with no additional “adhesive” layer added.
■ RESULTS AND DISCUSSION The SMP described above forms the basis for a not only strong but also highly reversible dry adhesive when its shape fixing and recovery capabilities are combined with a micropatterned surface design.13 Evenly spaced microscale pyramids − termed microtips − are patterned onto an SMP surface using a reusable silicon mold (see the Supporting Information). In the
Received: June 25, 2013 Accepted: August 14, 2013 Published: August 14, 2013
© 2013 American Chemical Society 7714 dx.doi.org/10.1021/am402479f | ACS Appl. Mater. Interfaces 2013, 5, 7714−7717
fabrication of our SMP surface, we chose a particular thermoset epoxy-based SMP that experiences a change in elastic modulus from approximately 2.5 GPa (below 35 °C) to 10 MPa (above 65 °C) corresponding to the SMP’s Tg.
14 As with most polymers, curing it in a mold captures surface details down to the nm (see the Supporting Information, Figure 3). A small section of this SMP in its rigid permanent shape is represented in Figure 1a. When heated above its Tg, it will become
compliant (Figure 1b) and can be easily deformed to a temporary shape. This is depicted in Figure 1c, where the SMP is pressed against a mating substrate, thereby compressing the microtips and causing the flat region between them to collapse into contact with the substrate. Note that an essential step toward forming a strong adhesive bond has been accomplished by this collapse; namely, the generation of large contact area between SMP and substrate. However, the bond is not yet very strong or stable. If pressure is released, the heated SMP, like any other elastically deformed compliant material, is susceptible to peeling failure and will try to spring back to its original shape. It is at this stage that the SMP sets itself apart from other common materials by locking in its temporary shape through cooling below its Tg (Figure 1d). The SMP will stay in this shape until it is again heated to resume its original shape, as shown in Figure 1e where the contact area, and therefore the adhesion, is nearly completely eliminated. Scanning electron micrographs of the fabricated microtipped SMP in both its permanent and temporary shapes are shown in images a and b in Figure 2, showing the microtips partially flattened and level with the collapsed intermicrotip region, all of which now make intimate contact with the substrate. The collapsed, temporary shape is reproduced using finite element software (see the Supporting Information) and is shown in Figure 2c, d along with the stress profile showing stresses concentrated near the microtips where deformation is greatest. There is a minimum microtip height that is required to
reliably cause the intermicrotip region to fully delaminate when the SMP is reheated. This height is a function of the SMP storage modulus, work of adhesion to the substrate material, detachment temperature and microtip spacing.13 In our case, the substrate material is glass and a target detachment temperature of 90 °C is selected for consistency with previous work.4,11 The stresses and strains generated during bonding near the microtips increase with microtip size, shown in Figure
3 with 100 μm spacing. Cooling below Tg traps these stresses internally within the polymer’s molecular structure, eliminating the restoring force between SMP and substrate. When reheated, the stresses will be relieved and the restoring force reestablished. For delamination between SMP and substrate to occur, the released strain energy must exceed the work of adhesion of the contacting area. Experimentally, the size, measured by base-width, required for reliable delamination from glass was determined to be between 18 and 21 μm. FEM analysis was performed with the storage modulus of 10 MPa14
and the work of adhesion of 46 mJ m−2 measured using atomic force microscopy (see the Supporting Information). FEM results shown in Figure 3 indicate the critical size to be between 15 and 18 μm; a consistent result given the idealizations inherent in computational analysis (see the Supporting Information). The adhesive strength and reversibility of the resulting
microtip SMP surface to a glass substrate is demonstrated in Figure 4. First, the unpatterned face (back side) of a 6.35 mm diameter section of SMP is glued to an aluminum cylinder to provide a means of loading and unloading the SMP surface (see the Supporting Information, Figure 1). The microtip SMP surface is then bonded to a glass-topped 5 kg mass using the process described in Figure 1a−d. The SMP-to-glass interface can support the full weight of the 5 kg mass as it is lifted and held, representing an adhesive strength of more than 156 N cm−2. To reverse the adhesion, the load is removed and the SMP heated to 90 °C to initiate shape recovery. The adhesion is now essentially zero, as in Figure 1e, and the SMP is easily lifted away from the glass surface. To quantify the adhesion, we performed tests using similarly
constructed SMP samples with an aluminum holder. The bonding of the rigid aluminum to the side opposite to the adhesive interface of the SMP was found to have unintended consequences for the observed collapse behavior. Heating and applying pressure to the SMP during bonding causes radial expansion in our cylindrical SMP adhesive; however, this expansion cannot occur where bonded to the aluminum, and so a slight convex curvature develops on the adhesive and the contact pressure for adhesion cannot be perfectly even from center to edge (see the Supporting Information,